The Study of the Surface Plasmon Polaritons at the Interface Separating Nanocomposite and Hypercrystal

: Surface plasmon polaritons (SPPs) propagating at the interfaces of composite media possess a number of fascinating properties not emerging in case of conventional SPPs, i.e., at metal-dielectric boundaries. We propose here a helpful algorithm giving rise for investigation of basic features of complex conductivity dependent SPPs at the interface separating nanocomposite and hypercrystal. The main goal of the work is to investigate dispersion of the SPPs propagating at the boundary separating two different media. Aiming to achieve the aforementioned goal that the effective Maxwell Garnett model is used. It is demonstrated that the SPPs dispersive properties are dramatically affected by the material conductivity. Correspondingly, the ﬁlling ratio of the nanoparticles in the composite and their dielectric properties also allow one to engineer characteristics of the SPPs. Having a deep insight into the conductivity dependent functions, we concluded, on their behavior for the case of hyperbolic regime and Dyakonov surface waves case. Our model gives rise for studying features of surface waves in the complex conductivity plane and provides more options to tune the fundamental features of SPPs at the boundaries correlated with composite media. Author Contributions: Conceptualization, T.I. and T.G.; methodology, T.I.; software, T.G.; valida-tion, T.G. and E.R.; formal analysis, E.R.; investigation, T.I.; resources, E.R.; data curation, T.G.; writing—original draft preparation, T.I.; writing—review and editing, T.G. and E.R.; visualization, supervision, T.G.; project administration, E.R.; funding


Introduction
During the last decades plasmonics attracted significant attention as the novel field pivoting the way for modern technologies, such as spectroscopy and sensing [1] and optical tweezers [2]. Surface plasmons (SPs) are introduced as the collective oscillations of the delocalized electrons presenting at metal-dielectric interfaces. SPs open the wide avenues to escape the diffraction limit of conventional optics [3] because of their capability to confine light in subwavelength dimensions with high efficiency. Doing so, the previous provides a fertile ground for a broad spectrum of applications ranging from surface enhanced spectroscopy [4], biomedical sensing [5] and solar cell photovoltaics [6] to optical antennas [7]. It is worthwhile noting that surface-plasmon-based circuits are established to bridge the disciplines of photonics and electronics at the nanoscale. The former allows to escape the current problems associated with the large size difference between the micrometer-scale bulky components of photonics and the nanometer-scale electronic chips.
The resonant oscillations of free electrons at the interface of nanocomposite media due to optical radiations give rise to surface plasmon polaritons (SPPs) [8]. The propagation of SPPs in nanocomposites has been extensively studied in [9][10][11]. Composite media with metal nanoparticles are of particular importance aiming to create nanostructured metal-insulator systems and novel approaches of manipulating light based on them. The emerge of transparent conductive oxides (TCOs) has attracted tremendous interest within the scientific community. These stand for as the alternative approach for plasmonics [12] in the near-infrared region. In contrary to noble metals, TCOs such as indium tin oxide (ITO) demonstrate a great tunability of their optical and electronic properties [13]. The former is possible via doping and electric bias. The construction and fabrication of ultracompact electroabsorption modulators [14] and for the proposal of new multimode modulator architectures [15] has benefited from the option of actively switching between a low-loss dielectric regime and a high-absorption plasmonic regime.
In the present work, we discuss complex conductivity of the medium, which dramatically affects tunability of SPPs. The obtained results may have significant applications in storage and sensing devices. Herein, we provide a detailed study of SPPs characteristics at the interface separating a nanocomposite and hypercrystal. Engineering properties of the nanocomposite and that of hypercrystal, the SPPs properties are tuned significantly. We present a complete description of the SPPs dispersion relation with different controlling parameters. Our study is extended aiming to examine the complex conductivity dependent properties.

Materials and Methods
Herein, we deal with the plane boundary separating a nanocomposite (NC) semiinfinite layer, which fills the half-space x < 0 and adjacent to it, hypercrystal filling the half-space x > 0 ( Figure 1). It should be stressed that the surface waves under consideration propagate along z axis. It is worthwhile noting that the structure under the study can be constructed by means of molecular beam epitaxy [16], chemical vapor deposition, atomic layer deposition and sacrificial etching [17]. The nanocomposite is presented as a nonconductive transparent matrix with a permittivity εn, in the volume of which regularly distributed semiconductor nanoparticles with permittivity εm. The frequency dependent dielectric function of the TCO based nanoparticles is of particular interest. An emergence of high-conducting metal being transparent has opened wide avenues recently. The issue has attracted lots of interest within the scientific community because of the metal being opaque for light. From the perspectives of the potential applications, transparent conducting metals described by high DC conductivity (σDC) are anticipated for optoelectronic devices, ranging from solar cells to electronic paper, touch screens and displays. Though, sity ne, a high-conducting metal (with a high ne) is certainly opaque for light because of its permittivity ε being typically very negatively affected by its high ωp. Conventional techniques to produce transparent conducting metals include the decrease of the ne, by utilizing transparent conducting oxides (TCOs). The parameters of the Drude-Lorentz approach for aluminum-doped zinc oxide (AZO), Ga-doped ZnO (GZO) and indium tin oxide (ITO) gained from experimental data [12] are presented in Table 1. Table 1. Drude-Lorentz parameters of plasmonic materials obtained from experimental data. One may approximate the materials dielectric function by the complex dielectric function: , with the values of the parameters outlined in the table [18]. Here εb is the polarization response from the core electrons (background permittivity), ωp is the plasma frequency, γp is the Drude relaxation rate.  The dielectric function of metallic medium in the complex conductivity and frequency domain is written as [19]:

AZO
where χ is the susceptibility of the system, σ is absolute value of complex conductivity and φ is its phase.
The dispersion relation of SPPs at a planar interface between the dielectric medium and metal forming a simple plasmonic structure in the complex conductivity and frequency domain is written as [20]: where εd is the permittivity of the host material. By making a step forward towards complex nanostructures, we made an assumption that the wavelength and the electromagnetic field penetration depth in the material are much larger that the size of inclusions suspended in a dielectric matrix. It is worthwhile mentioning that effective Maxwell Garnett model can be employed aiming to characterize the optical properties of the nanocomposite under consideration. The former approach is possible, if the interference effects of the inclusions are neglected and their volume fraction is as small as 1/3. Thus, one may apply the homogenization procedure and the effective complex permittivity of the nanocomposite can be expressed as follows where εn is the permittivity of the host material of the nanocomposite and f is the number of nanoparticles in the matrix. Based on the effective medium approximation one may calculate the effective permittivities of the anisotropic nanowire metamaterial (hypercrystal) according to [21]: where εd is the permittivity of the host material, εm is the permittivity of the inclusions embedded into the host material and ρ is the metal filling fraction ratio, which is calculated as: nanowire area unit cell area The metal filling fraction (ρ) is calculated based on the values of the pore diameter (d) and spacing (S) (Figure 1b). By taking into account a perfect hexagonal structure, the equation [22,23] is applied as follows: Based on this assumption one may derive a dispersion relation for the surface modes propagating at the interface between two anisotropic media. It is of particular importance to obtain a single surface mode with the propagation constant [24] by calculating the tangential components of the electric and magnetic fields at the interface By substituting (3)-(5) in (8), one may result in the dispersion relation as follows: , , ε σ ω σ ω ε σ ω ε σ ω ρ ε ρ β σ ω ε σ ω ρ ε ρ σ ω ε σ ω ε ρ ε σ ω ρ ε ρ ε σ ω ρ It is worthwhile noting, that Equation (9) stand for as the analytical expression of the dispersion relations investigated in the frame of the present work.

Results
The propagation of SPPs at the boundary of nanocomposite and hypercrystal is investigated. The absolute value of complex conductivity σ varies from 0 to 6 × 10 7 S/m.
Herein, the permittivity components of a hypercrystal and nanocomposite versus frequency are studied numerically aiming to identify the frequency ranges of Dyakonov surface waves (DSWs) and SPP waves existence (Figure 2). In the frequency ranges below the frequency ω||0 [25] the semiconductor-dielectric metamaterial possesses hyperbolic properties. It is worthwhile noting that in this frequency range the presence of conventional surface plasmon polaritons waves with propagation parallel to the optical axis is feasible under specific conditions. One may conclude from Figure 2

Conclusions
In conclusion, the SPPs properties were investigated versus conductivity at the interface of nanocomposite and hypercrystal. The amplitude of complex conductivity significantly influenced the SPPs propagation. The real part of SPPs dispersion relation was very large in comparison with the value of the free space wave-vector Re(β) > k0. It is worthwhile mentioning that propagation of SPPs was achieved at the interface with variation of complex conductivity. The conducted study allows one to conclude on the conditions of surface waves propagation in the complex conductivity plane. Thus,